ContentsIntroduction . . . . . . . . . . . . . . . . . . . . 2 Materials . . . . . . . . . . . . . . . . . . . . . . 2 Basic Guidelines . . . . . . . . . . . . . . . . . 2 Equipment . . . . . . . . . . . . . . . . . . . . . 2 Common Extrusion Issues . . . . . . . . . . 3 Polyurethane Films . . . . . . . . . . . . . . . 3 Cast Film and Sheet Extrusion . . . . . . . 3 Extrusion Coating . . . . . . . . . . . . . . . . 4 Blown Film . . . . . . . . . . . . . . . . . . . . . 4 Wire & Cable Coating, Hose Jacketing . . . 5 Tubing and Profile Extrusion . . . . . . . . . 6 Trouble Shooting Guide . . . . . . . . . . . . 7
be necessary to assure good processing. If a masterbatch or regrind/recycle are added to Estane TPU, then these materials must also be properly dried and may have a significant impact on the quality of the product. TPUs do not draw down well compared to other thermoplastics like polyethylene, therefore, drawdown should be minimized in the process. It is not recommended to shut a line down on TPUs. Even during short breaks, material should be kept moving at slow rates through the system.
EquipmentDehumidifying Hopper DryerIt is imperative to dry the material immediately prior to extrusion. This includes all raw materials containing TPU. Best results are obtained with 0.02% or less moisture content. Because of the relatively high consumption rate of an extruder, a good dehumidifying hopper drier is a preferred method for delivering consistently pre-dried and pre-heated material to the feed screw. The inlet air to the hopper should be checked at intervals for both dryness and temperature. For most extrusion grade Estane TPU products, the hopper should be sized so that all of the feed has been subjected to a minimum of two hours of dehumidified, dried air at 220F (105C) for 2-3 hours. A device to measure actual moisture content of the resin is recommended since dryer malfunctions can occur. Refer to individual technical data sheets for specific drying recommendations.
IntroductionDemand is continuously expanding for specialty materials that have a combination of outstanding mechanical properties together with the capability of being converted on conventional thermoplastic processing equipment. The family of Estane thermoplastic polyurethanes occupies a unique position of meeting this demand by providing a versatile range of grades from 70A Durometer to 65D Durometer that are being extruded commercially as wire and cable jacketing, hose jacketing, profiles, tubing, film & sheet, and fabric coatings. This bulletin is intended to provide general guidelines for equipment, procedures, and extrusion conditions that will help the customer obtain the best possible performance from Lubrizols line of Estane TPU extrusion grades. Additional information can be obtained by contacting your Lubrizol technical service or sales representative.
Most extruders are electrically heated with either band-type resistance heaters, cast-in block heaters or tubular resistance heaters wrapped around the barrel as seen in Figure 1. An efficient barrel cooling system is important to control the tendency for mechanical shear heat developed in the melt to override the electrical heater controls.Figure 1: Extruder
MaterialsPolyether polyurethanes are normally selected over polyester polyurethanes where end-use applications need hydrolytic stability, low temperature flexibility or fungal resistance. Although the polyether polyurethanes are inherently better in these characteristics, the hydrolytic stability and fungal resistance properties of polyester polyurethanes can be significantly improved by additive compounding. Softer Estane TPU compounds have no definite melting point, but soften gradually on heating, very much like flexible vinyl. They do achieve a fluid state characteristic of low-density polyethylene at temperatures well below the point of degradation. Initial softening points range from 250F-340F (121C-171C). Recommended processing conditions can be found in the product data sheets. Temperatures in excess of 450F (232C) may result in polymer degradation as evidenced by bubble formation. If this occurs, a reduction in zone temperatures will restore bubble-free extrudate and stabilize extrusion conditions.
The optimal extruder barrel length for Estane TPU is 30-32 times its internal diameter (30:1 L/D, 32:1 L/D). Although shorter barrels can be used, mixing efficiency and melt uniformity are not optimal. Cooling to the extruder feed throat is critical to prevent surging or bridging. Internal cooling to the screw is not needed.
Basic GuidelinesEstane TPU must be properly dried before processing. Inadequate drying results in a loss of properties and may give a poor appearance. Extruder barrel and die temperatures must be set properly for each product. Deviation from Lubrizols recommendations may result in poor extrusion quality. These recommendations can be found on the technical data sheet. The rate of extrusion has a large impact on the quality of the product and should be adjusted accordingly. TPUs in general can be tacky during processing, so rollers should be coated with suitable nonstick materials. Many Estane TPU compounds are already formulated to reduce blocking and tackiness. However, the addition of a lubricant masterbatch may2
Optimum screw design for extruding Estane TPU is still under further investigation. Excellent quality product has been obtained consistently with screws having the following characteristics: Barrier screw construction Compression ratio of 3:1 Long transition section (30-45% of screw length) Long metering section (30-45% of screw length) Hard-chrome, pinhole free, highly polished surface Clearance between screw and barrel liner of 0.003-0.005
A properly designed screw should melt and homogenize the Estane TPU material completely and develop a melt temperature about 10F below the recommended melt temperature. Barrier type screws will give the best quality output and several designs have been used successfully. A mixing section is also recommended at the end of the screw. The best performance seen has been with the Saxton and pineapple type mixers. The design recommendations for a series of 30:1 screws are listed in Table I. Proper maintenance of the screw will pay off in higher quality output, quicker start-ups, better output rates, and more reliable run-to-run performance consistency.
representative. Save a sample of the problem lot and a lot that worked on your process. Note that cloudy contaminants are a separate issue that should be reviewed with a Lubrizol representative.
Streaks or die lines: These are generally caused by build-up
in the die or damage to the die. You will likely need to clean your die. Best results are obtained by shutting down on a non-TPU resin like polyethylene.
Sticking or blocking: TPUs are generally tacky. Insure that the
proper formulation is being fed to the extruder. Check the coating on your rollers. A non-stick coating is required and can be damaged over time.
Suggested Screw Design for Extrusion of Estane Thermoplastic Polyurethanes Extruder Size Recommend Horse Power L/D Ratio Feed Section - number of flights Feed Section - flight depth Transition Section - number of flights Metering Section - number of flights Metering Section - flight depth Mixer - number of flights Compression Ratio Cored for Temperature Control Hard Chrome; Pinhole-Free; Polished 11/2" 25 30/1 8 0.270 10 9 0.090 3 3.0:1 No Yes 21/2" 50 30/1 8 0.360 10 9 0.120 3 3.0:1 No Yes 31/2" 100 30/1 8 0.450 10 9 0.150 3 3.0:1 No Yes 41/2" 200 30/1 8 0.525 10 9 0.175 3 3.0:1 No Yes
Non-uniform thickness in the machine direction: Check the extruder output for
surging. If the output is stable, you may be experiencing draw resonance. Reduce the drawdown. If this is not possible, attempt to heat up the melt and die. It may be necessary to switch to a lower molecular weight lot.
Non-uniform thickness in the transverse direction: This is seldom a resin issue.
Insure that the adjusting bolts are properly set. Check your system for build-up. Check for non-uniformity in cooling. There is a detailed troubleshooting guide at the end of this Processing Guide.
Breaker Plate & Screen
The primary function of the screen pack is to filter contaminants out of the plastic melt (e.g. paper, wood, metal, undispersed fillers, etc.). Screens should be constructed from stainless steel wire for strength and corrosion resistance. Normally a screen pack makeup of 20-40-80-20 mesh screens is optimal. However, some processes have used up to 200 mesh with good results. The breaker plate not only supports the screen pack, but also serves as a mechanical seal between the barrel and the adapter to the die. The holes in the breaker plate are normally 1/8 to 1/4 with a chamfer designed to give minimal obstruction to material flow.
As a film, TPU is soft but very tough. It can be made by blowing, extrusion casting, solution casting, or by calendering. It has a very high tear strength, high abrasion resistance and is extremely resistant to oils and greases. This combination of properties has led to its use for specialized packaging in the industrial and military fields, including the short-term storage of potable water. Other applications include the packaging of parts requiring storage in grease or oil where the films grease resistance, toughness, and clarity are important.
Cast Film and Sheet ExtrusionProcedure: The process for extruding film and sheeting isillustrated in Figure 2. Estane TPU pellets are compacted and melted in the extruder barrel. The high viscosity melted material is forced through a properly designed